Density of Phonon States at the Fe Sites in Superconducting FeSe as Function of Temperature and Pressure Vadim Ksenofontov 1 , Gerhard Wortmann 2 , Aleksandr Chumakov 3 , Teuta Gasi 1 , Sergey Medvedev 1,4 , Tyrel M. McQueen 5 , Richard J. Cava 5 , and Claudia Felser 1
Density of Phonon States at the Fe Sites in Superconducting FeSe as Function of Temperature and Pressure
Vadim Ksenofontov1, Gerhard Wortmann2, Aleksandr Chumakov3, Teuta Gasi1, Sergey Medvedev1,4, Tyrel M. McQueen5, Richard J. Cava5, and Claudia Felser1
1Institut für Anorganische und Analytische Chemie, 55099 Mainz, Germany
2Department Physik, Universität Paderborn, 33095 Paderborn, Germany
3ESRF, 38043 Grenoble, France
4Max-Planck-Institute for Chemistry, 55128 Mainz, Germanyy
5Department of Chemistry, Princeton University, Princeton NJ 08544, USA
Oral Contribution on the HFI-NQI 2010 at CERN, Geneve, 13.-17.Sept. 2010
- Superconducting (s.c.) Fe1+xSe: phase analysis
- Pressure-induced effects in Fe1.01Se:
Superconductivity, structure, Mössbauer spectra
- Temperature and pressure dependence of the density of phonon states at the Fe sites in Fe1.01Se
- Comparison with the phonon-DOS in s.c. FeSe0.5Te0.5 X-tals: Use of polarisation
- Short discussion of possible pairing mechanism in FeSe systems
Refs: F.C. Hsu, Proc. Natl Acad. Sci. 105, 14262 (2008). T.M. McQueen et al., Phys. Rev. B 79, 014522 (2009).
S. Medvedev et al., Nature Mater. 8, 630 (2009).
Susceptibiliy and 57Fe-ME studies
T.C. McQueen et al., PRB 79, 014522 (2009).
- Superconductivity (s.c.) in FeSe systems depends sensitively on stoichiometry
- No significant differences in 57Fe-ME spectra between –Fe1.01Se and –Fe1.03Se
- Both s.c. and non-s.c. samples are non-magnetic, no sign of magnetic ordering
D = 270(5) K
D = 290(5) K
Normalized area under Mössbauer spectra
is sensitive to the tetra.-orthor. transition.
Fe binding is slighty softer in orthor. phase.V. Ksenofontov et al., unpublished.
- XRD scans of the (220) reflection in Fe1.01Seshow the appearance of the orthorhombic distortion.- This subtle distortion is not reflected in the 57Fe- Mössbauer quadrupole spectra.
T.M. McQueen et al., PRL 103, 057002 (2009). .
Resistivity and Mössbauer FeSe as Function of Temperature and Pressure
spectra of Fe1.01Se
under high pressure
Tc increases from 8.5 K (0 GPa) to 36.7 K at 8.9 GPa
Very steep initial increase:Tc/ p = 12.6(8) K/GPa
Ref.: S. Medvedev et al., Nature Mater. 8, 630 (2009)
Short History of Nuclear Resonant Scattering of SR FeSe as Function of Temperature and Pressure
1958: Detection of the Mössbauer effect by Rudolf L. Mößbauer
1974: Proposal: Use of SR for MS by Stan Ruby
1985: Nuclear Bragg Scattering with SR by Erich Gerdau, Rudolf Rüffer et al.
1991: Nuclear Forward Scattering, NFS (SMS) J.B. Hastings et al.
fast detectors (ns)
1995: NFS under pressure (H.F. Grünsteudel et al.)
Magnetism in the Mbar range in RFe2 (Rainer Lübbers et al.)
1995: Nuclear Inelastic Scattering, NIS: M. Seto, W. Sturhahn, E.E. Alp
Phonons in iron under pressure with NIS:2000: R. Lübbers et al., up to 40 GPa, ESRF2001: H.-K. Mao et al., up to 153 GPa, APS
HP with 57Fe,119Sn,149Sm, 151Eu, ..
NFS and NIS of synchrotron radiation FeSe as Function of Temperature and Pressure
NFS: determination of hyperfine interactions
NIS: determination of the local phonon DOS at the Mössbauer atom
57Fe-NIS studies performed with a resolution of 0.75 meV at 14.4 keV at beamline ID18 of ESRF
57Fe-NIS spectra of Fe1.01Se at 295 K (full circles) and at 10 K (open circles)V. Ksenofontov, G.W., A.I. Chumakovet al., PRB 81, 184510 (2010)
Fe phonon-DOS in FeSe compared with FeSe FeSe as Function of Temperature and Pressure0.5Te0.5 X-tals**100% enriched in 57Fe, from V. Tsurkan, J. Deisenhofer, A. Loidl (Univ. Augsburg)
Optical modes adjusted by 5 Gaussians (#4-9): PRB 81, 184510 (2010).
FeSe at 10 K, polycryst. sample with textureTC = 8 K
By Te substitution, strong shiftof all modes to lower energy, caused by combined (not additive) effcts of: - lattice expansion of ~10% (negative pressure of ~5 GPa) - increase of the effective mass m* by ~8%. All spectral features of FeSe present, but with strong polari-sation dependence, allowing an assignment of modes.
Spectral features are broadened
by Te substitution and by higher temperature (296 K).
V. Ksenofontov et al., unpubl.
FeSe0.5Te0.5 X-talk // c, 296 KTC = 14 K
FeSe0.5Te0.5 X-talk // ab, 296 K
TC = 14 K
FeSe0.5Te0.5 polycryst sample with strongtexture, as evident from X-tal sample with c-axis.
Same principal behaviour as for T-dependent phonon-DOS of FeSe:
(i) sharpening of spectral features and (ii) shift to higher energies by ~4% by loweringtemperature from 295 K to 10 K.
Subtle changes in phonon-DOS above/below Tc = 14 K and above below tetr./orthorh. p.t. are still under investigation.
V. Ksenofontov et al., in preparation.
D,LT = (3/a)1/3/kB
Fe-partial phonon-DOS, g(E)/E2 for Fe1.01Se at 295 K, demonstrating for the low-energy range the strong modification of the lowest acoustic mode at 5 meV under pressure, attributed to vibrations along the “soft” c-axis.
- Fe-partial phonon-DOS, g(E)/E2, for FeSe0.5Te0.5 at 295 K, demonstrating the strong modification of the acoustic modes in different X-tal directions: - The “soft” mode, now at 4.5 meV, reflects the high c-axis compressibility.
-Preliminary evaluation, shown is the projected phonon-DOS with g(E) ~cos2(k,c)
FeSe as Function of Temperature and PressureD
= 285(4) K
0.1 - Coulomb pseudopotential
8.0 K corresponds to
0.65(1)Pressure effect on Tc in Fe1.01Se
Electron-phonon coupling constant ~ <ω-2>
Theory: = 0.1 (D. J. Singh)
Experiment: = 0.21 for LaOFeAs (L. Boeri)
= 1.3 for PrFeAsO1-xFx (D. Bhoi)
A. Subedi, L. Zhang, D.J. Singh, M.H. Du, Phys. Rev. B 78, 134514 (2008).
L. Boeri, O.V. Dolgov, and A.A. Golubov, Phys. Rev. Lett. 101, 026403 (2008).
D. Bhoi, P. Mandal, and P. Choudhury, Supercond. Sci. Technol. 21, 125021 (2008).
Acknowledgements: FeSe as Function of Temperature and PressureUni Mainz (Inst. Anorg. Analyt. Chemie): Vadim Ksenofontov, T. Gasi, F. Casper, Claudia FelserMPI Chemistry Mainz:Sergej Medvedev, I.A. Trojan, T. Palayuk, M.I. EremetsDepartment Chemistry, Princeton:Tyrel M. McQueen, R.J. Cava (Fe1.01Se samples)Institut Physik, Uni Augsburg:V. Tsurkan, J. Deisenhofer. A. Loidl (FeSe0.5Te0.5 samples) Thank you for your attention